advertisement

International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net Prediction of Compressive Strength of High Performance Concrete using Artificial Neural Network (ANN) Models K. Kaviya1, J. Premalatha2 1P.G Scholar, Kumaraguru College of Technology, Coimbatore. in Civil Engineering Department, Kumaraguru College of Technology, Coimbatore, Tamilnadu, India. ---------------------------------------------------------------------***---------------------------------------------------------------------2Professor Abstract - Concrete is the most versatile construction material because it can be designed to withstand harshest environments. Nowadays, most concrete mixture contains supplementary cementitious materials (SCM) which form a part of the cementitious component. The main benefits of SCMs are their ability to replace certain amount of cement and still be able to display cementitious property, thus reducing the cost of using Portland cement. The fast growth in industrialization has resulted in tons and tons of by-product or waste materials such as Fly Ash, Silica Fume, Ground Granulated Blast Furnace Slag, Steel fibers, etc., which can be used as SCMs in concrete. In the present work, a model has been developed using Artificial Neural Network (ANN) and Multiple Regression Analysis (MRA for the prediction of compressive strength of concrete with SCMs like Fly Ash, Silica Fume and Ground-Granulated Blast Furnace Slag (GGBFS). Experimental data published by various authors have been used for training, validation and testing process in the model development. The mix contents like cement, flyash water cement ratio, GGBS, silicafume are taken as the input parameters and cube compressive strength of the concrete was considered as the target output parameter. The data sets were modelled using both MRA and ANN and their results were compared. Three types of algorithms, Bayesian Regularization Algorithm, Levenberg-Marquardt Method and Scaled Conjugate Gradient Method were used in the study. The models using Bayesian Regularization Algorithm and Levenberg-Marquardt Method are found to be optimum model with the regression coefficients of 0.97 and 0.94 respectively. The model developed using Multiple Regression Analysis has a regression value (R) of 0.74 and does not give accurate results and hence this method is discarded. with these cementitious materials are used extensively throughout the world. Some of the major users are power, gas, oil and nuclear industries. The applications of such concretes are increasing with the passage of time due to their excellent performance, low influence on energy utilisation and environment friendliness. In order to minimize the experimental task for concrete mix design, probabilistic models are generally constructed using Artificial Neural Networks (ANN) and Multiple Regression Analysis (MRA) and constitutive equations are derived. Multiple Regression Analysis (MRA) is one of the traditional methods used to forecast the compressive strength of concrete, by implementing linear or non-linear method. MRA is based on the least-squares fit approach. It is a statistical technique to examine the relationship between one or more independent variables and a dependent variable. Neural networks are networks of many simple processes, which are called units, nodes, or neurons, with dense parallel interconnections. The connections between the neurons are called synapses. Each neuron receives weighted inputs from other neurons and communicates its outputs to other neurons by using an activation function. Thus, information is represented by massive cross-weighted inter-connections. Neural networks might be single-or multi layered. The single-layer neural networks present processing units of the neural networks, which take input from the outside of the networks and transmit their output to the outside of the networks; otherwise, the neural networks are considered multi layered. The basic methodology of neural networks consists of three processes: Network training, testing, and implementation. Key Words: Supplementary cementitious materials, Artificial Neural network, Multiple regression analysis. In this study, multilayer preceptor (MLP): a feed forward artificial neural network model is implemented. A large test database has been extensively surveyed and collected. It is then carefully examined to establish the input vectors and the desired output vectors. Finally, a new model is proposed based on ANN and then verified against experimental data which has been collected from different sources. 1. INTRODUCTION High-Performance Concrete (HPC) refers to the type of concrete mixture which has adequate workability, develops high strength and possesses excellent durability properties throughout its intended service life. To ensure eco-friendly and sustainable development, several industrial by-products such as Fly ash, Silica fume, GGBS, Fibers etc., are being utilized in concrete manufacturing as a substitute for either cement or fine aggregate or as an admixture. The mineral materials, when used in HPC, can enhance either or both the physical and durability properties of concrete. Concretes © 2019, IRJET | Impact Factor value: 7.211 ANN has the tendency to exploit non-linearity, predict input–output relationship, adapt to the changes in the free parameters and has sufficient fault tolerance. In the current study, the compressive strength of High Performance | ISO 9001:2008 Certified Journal | Page 1378 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net Concrete is taken as the dependent variable, whereas, the mix constituents and age of the specimen form the independent variables. the compressive strength (fc) obtained from various literature collected for this work are given through Table 1 to Table 6. Bhanja and Sengupta (2005) worked on Influence of silica fume on the tensile strength of concrete. Extensive experimentation was carried out over water–binder ratios ranging from 0.26 to 0.42 and silica fume–binder ratios from 0.0 to 0.3. For all the mixes, compressive, flexural and split tensile strengths were determined at 28 days.A. Elahi et al, carried out investigation to evaluate the mechanical and durability properties of High Performance Concrete (W/B = 0.3) containing supplementary cementitious materials (Silica Fume, Fly Ash, Ground Granulated Blast Furnace Slag) in binary and ternary systems. Portland cement was replaced with fly ash upto 40%, silica fume upto 15% and GGBS upto a level of 70%. The ternary mixes containing GGBS or Fly Ash (50%) and Silica Fume (7.5%) performed the best amongst all the mixes to resist the chloride diffusion. Silica fume (7.5%) performs better than other supplementary cementitious materials for the strength development.B. K. Raghu Prasad et al, proposed an artificial neural network (ANN) to predict 28 days compressive strength of high performance concrete. The high values of R2 demonstrated that the proposed ANN model was suitable for predicting the compressive strength values very closely with the experimental values. K. E. Hassan et al, carried laboratory study on the properties of super-plasticized high performance concrete by using SF and FA (10%, 30% by weight of cement). The SF concrete showed similar strength development to that of the Ordinary Portland Cement concrete but slight higher values at all tested ages (1, 3, 7, 28, 365 days). FA concrete gave lowest compressive strength at early ages, same at 28 days and higher at 365 days than OPC concrete.Vaishali G Ghorpade performed tests on four mixes of concrete with 0%, 0.5%, 1.0% and 1.5% by volume fraction of glass fiber, silica fume (0%, 10%, 20%, 30% by weight of cement) with W/B ratio = 0.35, aggregate/binder = 2.0 and super-plasticizer 1% of the weight of cement. The optimum percentage recommended as 1% fiber volume with 10% silica fume for achieving maximum benefits in compressive strength, split tensile strength and flexural strength. 4. CREATION OF ALGORITHM FOR ANN In order to develop ANN architecture, 466 samples of concrete data on 7th, 28th, 56th and 90th day of compressive strength of concrete were collected. In the present work, training data set comprises 326 data entries, and the remaining data entries (140) are divided between the validation and testing sets. To test the reliability of the neural network model, 70 samples were randomly selected as the test set and 70 samples as the validation set. The dividing process was carried out randomly between the three sets and each dataset has been statistically examined to ensure that it covers the range of input parameters. In a neural network if the area for data is more, learning is better. Table 7 – Maximum and Minimum values of data used in ANN Model Data Components Minimum Maximum 100.5 650 502 835 853 1848 Fly ash (kg/m3) 0 227 Silica fume (kg/m3) 0 147 GGBS (kg/m3) 0 325 14.2 119 Cement (kg/m3) Fine Aggregate (kg/m3) Coarse (kg/m3) Compressive (MPa) 2. OBJECTIVES The objective of this study is to construct probabilistic models for the prediction of compressive strength of High Performance Concrete with Fly ash, Silica fume and GGBS as partial cement replacement. Aggregate strength Table 8 – Parameters used in ANN Model Number of input layer neurons 8 3. INPUT AND OUTPUT DATA FOR ANN MODELLING Number hidden layer 1 The details on the materials used in various mixes like cement, fine aggregate (FA), Coarse aggregate (CA), water-cement (w/c) ratio and supplementary cementing materials such as flyash , slicafume and ground granulated blast furnace slag (GGBS) used in experimental works and Number of hidden layer neurons 30 Number of output layer neutron 1 © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1379 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net 4.1 Training of Network 4.3 Selection of Training Algorithm Feed-Forward Neural Network (FFNN) consists of at least three layers of neurons: an input layer, at least one intermediate hidden layer, and an output layer. Typically, neurons are connected in a feed-forward fashion with input units fully connected to neurons in the hidden layer and hidden neurons fully connected to neurons in the output layer. Back propagation is the traditional training method for FFNN during which the neurons adapt their weights to acquire new knowledge. Training of datas can be done by choosing an algorithm. There are three types of algorithms. Learning in FFNN with back propagation occurs during the training phase in which each input pattern from the training set is applied to the input layer and then propagates forward. The pattern of activation arriving at the output layer is then compared with the correct (associated) output pattern to calculate an error signal. The error signal for each such target output pattern is then back propagated from the output layer to the input neurons in order to adjust the weights in each layer of the network. After the training phase during which the NN learns the correct classification for a set of inputs, it can be tested on a second (test) set of samples to see how well it classifies new patterns. Thus, an important consideration in applying back propagation learning is how well the network makes the generalization. This algorithm typically takes more memory but less time. Training automatically stops when generalization stops improving, as indicated by an increase in the mean square error of the validation sample. i. Levenberg-Marquardt ii. Bayesian Regularization iii. Scaled Conjugate Gradient i) Levenberg-Marquardt Method Figure.1 Feed Forward Neural Network Diagram Figure .3 Plot Error Histogram for LevenbergMarquardt Method 4.2 Construction of Neural Network Model The architecture of a network describes how many layers a network has, the number of neurons in each layer, each layer’s activation function, and how the layers connect to each other. In the present study there are eight inputs and compressive strength of concrete is output. For this reason, the initial structure of neural network is illustrated Figure 1. Figure.4 Plot Regression for Levenberg-Marquardt Method Figure 2: Architecture of Neural network developed © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1380 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net testing. Some of the above mentioned input data sets are chosen for the prediction of compressive strength using ANN model. From observing the above three algorithms, Bayesian Regularization Algorithm yields the best fit results with least number of errors and Regression value (R) of 0.97, while Levenberg-Marquardt Method has a Regression value (R) of 0.94 and Scaled Conjugate Gradient Method has a Regression value (R) of 0.12. Hence, by training the inputs by Bayesian Regularization Algorithm the compressive strength of the concrete mixes is predicted by using ANN model. ii) Bayesian Regularization Method This algorithm typically takes more time, but can result in good generalization for difficult, small or noisy datasets. Training stops according to adaptive weight minimization (regularization). 6. DEVELOPMENT OF MODEL USING MRA Building a model is rarely a simple or straightforward process. Analysts must have a prior knowledge of the variables to identify as independent variables to be included in the model. The independent variables can be first-order or second-order terms, interaction terms, and dummy variables. The variable screening methods, stepwise regression and all-possibleregressions selection procedure, can help analysts to select the most important variables that contribute to the response variable. Figure.5 Plot Error Histogram for Bayesian Regularization Method i) 1) Stepwise Regression determines the independent variable(s) added to the model at each step using t-test. Scaled Conjugate Gradient Method 2) All-Possible-Regressions Selection Procedure gives all possible models at each step with the suggested independent variable(s). One drawback of adding more independent variables in the model will increase eventually to 1. Adjusted or MSE Criterion takes into account the sample size and the number of parameters in the model increases only if MSE decreases. The largest or smallest MSE indicates the best fit of the model. A small value indicates that the total mean square error and the regression bias are minimized. This algorithm takes less memory. Training automatically stops when generalization stops improving, as indicated by an increase in the mean square error of the validation sample. Figure.6 Plot Regression for Bayesian Regularization Method 5. RESULTS OF ANN MODEL The input data sets for ANN model were trained under the category of 70% training, 15% validation and 15% © 2019, IRJET | Impact Factor value: 7.211 Figure.7 Maximum Regression value curve | ISO 9001:2008 Certified Journal | Page 1381 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net 5.1 Results of Multiple Regression Analysis Next to the ANN model, Regression value is found using Multiple Regression Analysis. The Regression value (R) obtained here is 0.74. [4] 6. CONCLUSIONS [5] From the above results and test data, it is found that Artificial Neural Network model is best suited for the prediction of compressive strength of High Performance Concrete using Supplementary Cementitious Materials, when compared to Multiple Regression Analysis. The graph shows a marginal difference between actual and predicted values. Therefore, compressive strength values of concrete can be predicted in ANN models without attempting any experiments in a quite short period of time with marginal errors. [6] [7] Thus, it can be concluded that the application of ANN is more user friendly and more explicit model can be made which help the concrete industry to avoid the risk of faulty or deficient concrete that often entails durability and safety problems. [8] [9] fume as Admixture,” 35th Conference on OurWorld in Concrete & Structures, Singapore, 25-27 Au-gust 2010, pp. 1-8. K. E. Hassan, J. G. Cabrera and R. S. Maliehe, “The Effect of Mineral Admixtures on the Properties of High Performance Concrete,” Cement & Concrete Composites, Vol. 22, No. 4, 2000, pp. 267-271. J.A.Peter, M.Neelamegham “Utilization of fly ash as cement replacement material to produce high performance concrete” structural engineering research centres (CSIR) Chennai 1999. Patil Shreekedar.A and Kumbhar .P.D “Study on effect of mineral admixtures in mix proportioning of HPC”, International Journalof Research in Advent Technology”, Vol.1,Issue.5,pp.499-504,2013. B. K. Raghu Prasad, H. Eskandari and B. V. Venkatarama Reddy, “Prediction of Compressive Strength of SCC and HPC with High Volume Fly Ash Using ANN,” Construction and Building Materials, Vol. 23, No. 1, 2009, pp.117-128. Sudarsana Rao.Hunchate, Sashidhar.Chandupall, Vaishali.G.Ghorpode and Venkata Reddy.T.C “Mix Design of High Performance Concrete Using Silica Fume and Superplasticizer” International Journal of Innovative Research in Science, ISSN: 2319-8753. T.Shanmugapriya , 2,Dr.R.N.Uma, Experimental Investigation on Silica Fume aspartial Replacement of Cement in High Performance Concrete, The International Journal Of Engineering And Science (IJES) ||Volume||2 ||Issue|| 5 ||Pages|| 40-45||2013|| ISSN(e): 2319 – 1813 ISSN(p): 2319 – 1805. N. Venkateswarao and A. Dattatreya Kumar - Influence of Silica Fume and GGBS on Strength Characteristics of High Performance Concrete, Volume 06 Issue 09, September 2016 [11] P.Vinayagam,“Experimental Investigation on high performance concrete Using Silica Fume and Superplasticizer”, International journal of Computer and Communication Engineering, Vol.1, No.2, pp. 168171, 2012. [12] T.V.S. Vara Lakshmi, Prof. S. Adiseshu (05 February 2016), “A Study on Preparing Of High Performance Concrete Using Silica Fume and Fly Ash”. [10] Figure.8 Regression value curve of MRA REFERENCES Bhanja, B. Sengupta, “Influence of silica fume on the tensile strength of concrete”, Cement and Concrete Research, Vol. 35, (2005), pp. 743-747. [2] Elahi, P. A. M. Basheer, S. V. Nanukuttan and Q. U. Z. Khan, “Mechanical and Durability Properties of High Performance Concretes Containing Supplementary Cementitious Materials,” Construction and Building Materials, Vol. 24, No. 3, 2010, pp. 292-299. [3] V. G. Ghorpade, “An Experimental Investigation on Glass Fibre reinforced High Performance Concrete with Silica [1] © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1382 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net Table 1 - Mix Proportions containing Fly ash INPUT SOURCE OUTPUT Cement (kg/m3) FA (kg/m3) CA (kg/m3) w/c ratio Flyash kg/m3 fc (28 days) MPa 454 593 1848 0.35 80 94 428 593 1848 0.31 106 95 401 593 1848 0.4 135 94 374 593 1848 0.3 160 86 318 745 952 0.37 136 47 280 768 953 0.42 120 43 250 820 939 0.47 107 37 227 662 950 0.37 227 40 200 685 982 0.42 200 37 179 703 1008 0.47 179 30 Peter et.al 2009 Subbiah Karthick et.al Table 2 - Mix Proportions containing Silica fume INPUT SOURCE Uma et.al Venkateswarao et.al Sengupta et.al © 2019, IRJET | OUTPUT Cement (kg/m3) FA (kg/m3) CA (kg/m3) w/c ratio Silica fume kg/m3 fc (28 days) Mpa 532.35 672 1149.8 512.51 672 1149.8 0.34 13.8 60 0.34 27.59 61 492.66 672 1149.8 0.34 41.39 65 472.5 672 1149.8 0.34 55.19 60 453.6 672 1149.8 0.34 68.98 60 509.2 737 1044.0 0.32 26.8 65.77 482.4 737 1044.0 0.32 53.6 68 455.6 737 1044.0 0.32 80.4 65.33 494 667 1146.0 0.26 26 93 468 667 1146.0 0.26 52 92 442 667 1146.0 0.26 78 95 416 667 1146.0 0.26 104 92.5 390 667 1146.0 0.26 130 85 484.5 653 1122.5 0.3 25.5 75 459 653 1122.5 0.3 51 78 433.5 653 1122.5 0.3 76.5 82 408 653 1122.5 0.3 102 85 382.5 653 1122.5 0.3 127.5 81 475 640 1100.0 0.34 25 64 450 640 1100.0 0.34 50 70 425 640 1100.0 0.34 75 72 400 640 1100.0 0.34 100 75 375 640 1100.0 0.34 125 73 465.5 628 1078.0 0.38 24.5 59 Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1383 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 Venkata Reddy et. al Vivek, et.al Vishnura m et.al Sanjeewa et.al Suresh kumar et.al www.irjet.net 441 628 1078.0 0.38 49 63 416.5 628 1078.0 0.38 73.5 64 392 628 1078.0 0.38 98 65 367.5 628 1078.0 0.38 122.5 66 343 628 1078.0 0.38 147 64 456 616 1058.0 0.42 24 49 432 616 1058.0 0.42 48 55 408 616 1058.0 0.42 72 56 384 616 1058.0 0.42 96 57 360 616 1058.0 0.42 120 60 336 616 1058.0 0.42 144 48 486 773 1044.0 0.29 25.55 62.67 461 773 1044.0 0.29 51.1 65.33 436 773 1044.0 0.29 76.65 71.11 411 773 1044.0 0.29 102.2 67.33 386 773 1044.0 0.29 127.75 63.11 491.61 683.24 1108.13 0.32 12.6 55.24 478.99 683.24 1108.13 0.32 25.21 58.54 466.39 683.24 1108.13 0.32 37.81 62.12 543.31 599.81 1171.47 0.3 28.58 55 529.01 594.58 1171.47 0.3 42.87 61.33 514.72 589.35 1171.47 0.3 57.16 56.33 543.31 599.81 1171.47 0.32 28.58 63 529.01 594.58 1171.47 0.32 42.87 66 514.72 589.35 1171.47 0.32 57.16 60 522.5 543 1088.0 0.3 27.5 66.1 495 543 1088.0 0.3 55 69.7 481.3 543 1088.0 0.3 68.8 69.9 467.5 543 1088.0 0.3 82.5 64.4 420 663 1082 0.4 21 60 542.99 610.27 1171.8 0.45 28.58 55 514.41 610.27 1171.8 0.45 57.16 61.33 485.83 610.27 1171.8 0.45 85.74 56.33 Table 3 - Mix Proportions containing GGBS INPUT Cement (kg/m3) SOURCE N.Venkat eswarao et.al © 2019, IRJET | FA (kg/m3) OUTPUT CA (kg/m3) w/c ratio GGBS kg/m3 fc (28 days) MPa 482.4 737 1044 0.32 53.6 64.88 428.8 737 1044 0.32 107.2 66.22 375.2 737 1044 0.32 160.8 68.44 321.6 737 1044 0.32 214.4 65.33 375.2 737 1044 0.32 160.8 65.77 Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1384 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 Subbiah Karthick et.al www.irjet.net 318 762 946 0.37 136 48 280 783 972 0.42 120 42 250 835 956 0.47 107 39 227 760 943 0.37 227 50 200 780 969 0.42 200 45 179 832 853 0.47 179 40 Table 4 – Mix Proportions containing Fly ash and Silica fume INPUT SOURCE KantaRao, et.al Vara Lakshmi, et.al Ankit Kumar Sanjeewa et.al Suresh kumar © 2019, IRJET | OUTPUT Cement (kg/m3) FA (kg/m3) CA (Kg/m3) w/c ratio Flyash kg/m3 Silicafume kg/m3 fc (28 days) MPa 570 502 1060 0.32 30 60 82.1 540 502 1060 0.32 60 60 85 510 502 1060 0.32 90 60 91 480 502 1060 0.32 120 60 87 450 502 1060 0.32 150 60 83 420 502 1060 0.32 180 60 79 495.91 601.55 1151.06 0.26 58.34 29.17 67 481.33 601.55 1151.06 0.26 58.34 43.75 71 466.74 601.55 1151.06 0.26 58.34 58.34 81 452.16 601.55 1151.06 0.26 58.34 72.92 77 389.7 625 1164 0.43 8.66 34.64 41 389.7 625 1164 0.43 17.32 25.98 39 389.7 625 1164 0.43 21.65 21.65 37 389.7 625 1164 0.43 25.98 17.32 36.5 389.7 625 1164 0.43 34.64 8.66 36.5 495 543 1088 0.3 27.5 27.5 71.1 467.5 543 1088 0.3 55 27.5 70.8 440 543 1088 0.3 82.5 27.5 66.4 412.5 543 1088 0.3 110 27.5 62.9 467.5 543 1088 0.3 27.5 55 70.6 440 543 1088 0.3 55 55 68.7 412 543 1088 0.3 82.5 55 67.4 385 543 1088 0.3 110 55 65.6 453.8 543 1088 0.3 27.5 68.8 72.1 426.3 543 1088 0.3 55 68.8 70.1 398.8 543 1088 0.3 82.5 68.8 65.8 440 543 1088 0.3 27.5 82.5 65.8 412.5 543 1088 0.3 55 82.5 63 385 543 1088 0.3 82.5 82.5 61.2 485.83 610.2 1171.8 0.45 57.16 28.58 58.67 457.26 610.2 1171.8 0.45 57.16 57.16 57.64 428.68 610.2 1171.8 0.45 57.16 85.74 55.34 Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1385 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net Table 5 - Mix Proportions containing Fly ash and GGBS INPUT SOURCE Kavitha Chandrak ar, et.al Afroz Khan, et.al OUTPUT CEMENT (kg/m3) FA (Kg/m3) CA (Kg/m3) W/C RATIO FLY ASH GGBS fc (28 Days) MPa 419.99 585 1205 0.45 46.66 46.66 52 335.99 585 1205 0.45 83.99 46.66 54 326.66 585 1205 0.45 139.99 46.66 56 279.99 585 1205 0.45 186.66 46.66 60 419.99 585 1205 0.45 46.66 93.33 54 335.99 585 1205 0.45 83.99 93.33 56 326.66 585 1205 0.45 139.99 93.33 60 279.99 585 1205 0.45 186.66 93.33 62 419.99 585 1205 0.45 46.66 139.99 54 335.99 585 1205 0.45 83.99 139.99 62 326.66 585 1205 0.45 139.99 139.99 64 279.99 585 1205 0.45 186.66 139.99 70 419.99 585 1205 0.45 46.66 186.66 51 335.99 585 1205 0.45 83.99 186.66 52 326.66 585 1205 0.45 139.99 186.66 54 279.99 585 1205 0.45 186.66 186.66 62 390 695 981 0.2 104 156 93.13 390 695 981 0.2 117 143 96.7 390 695 981 0.2 130 130 100 357.5 695 981 0.2 117 175.5 91.25 357.5 695 981 0.2 131.63 160.87 90.45 357.5 695 981 0.2 146.25 146.25 96.23 325 695 981 0.2 130 130 95.15 325 695 981 0.2 146.25 146.25 94 Table 6 – Mix Proportions containing Silica fume and GGBS INPUT SOURCE Vivek, et.al Venkata Reddy Gorav Gupta, et.al © 2019, IRJET OUTPUT Cement (kg/m3) FA (kg/m3) CA (kg/m3) w/c ratio Silica fume kg/m3 GGBS kg/m3 fc (28 days) MPa 375.2 683 1060 0.32 26.8 160.8 68.44 375.2 683 1060 0.32 53.6 160.8 70.66 375.2 683 1060 0.32 80.4 160.8 68.88 348.4 737 1044 0.32 26.8 160.8 68.44 321.6 737 1044 0.32 53.6 160.8 70.66 294.8 737 1044 0.32 80.4 160.8 68.88 395.6 650 1130 0.4 12.9 21.5 32.01 374.1 650 1130 0.4 12.9 43 38.55 352.6 650 1130 0.4 12.9 64.5 37.25 331.1 650 1130 0.4 12.9 86 38.55 391.3 650 1130 0.4 17.2 21.5 40.3 | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1386 International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 Volume: 06 Issue: 04 | Apr 2019 p-ISSN: 2395-0072 www.irjet.net 369.8 650 1130 0.4 17.2 43 42.04 348.3 650 1130 0.4 17.2 64.5 44.22 326.8 650 1130 0.4 17.2 86 38.12 387 650 1130 0.4 21.5 21.5 48.15 365.5 650 1130 0.4 21.5 43 26.4 344 650 1130 0.4 21.5 64.5 35.91 322.5 650 1130 0.4 21.5 86 35.07 Table 8– Comparison of experimental results with ANN model results CEMENT (kg/m3) FINE AGGREGATE (Kg/m3) COARSE AGGREGATE (Kg/m3) W/C RATIO FLY ASH SILICA FUME 570 502 1060 0.32 30 540 502 1060 0.32 510 502 1060 0.32 480 502 1060 450 502 420 COMPRESSIVE STRENGTH (28 DAYS) Experimen tal data Prediucted value 60 82.1 87.1 60 60 85 87.5 90 60 91 86.4 0.32 120 60 87 87.4 1060 0.32 150 60 83 86.8 502 1060 0.32 180 60 79 79.3 495.91 601.55 1151.06 0.26 58.34 29.17 67 74.6 481.33 601.55 1151.06 0.26 58.34 43.75 71 74.7 466.74 601.55 1151.06 0.26 58.34 58.34 81 74.4 452.16 601.55 1151.06 0.26 58.34 72.92 77 73.7 389.7 625 1164 0.43 8.66 34.64 41 38.4 389.7 625 1164 0.43 17.32 25.98 39 38.3 389.7 625 1164 0.43 21.65 21.65 37 38.4 389.7 625 1164 0.43 25.98 17.32 36.5 38.5 389.7 625 1164 0.43 34.64 8.66 36.5 38.6 495 543 1088 0.3 27.5 27.5 71.1 72.8 467.5 543 1088 0.3 55 27.5 70.8 71.6 440 543 1088 0.3 82.5 27.5 66.4 66.9 412.5 543 1088 0.3 110 27.5 62.9 63.5 467.5 543 1088 0.3 27.5 55 70.6 70.4 440 543 1088 0.3 55 55 68.7 68.7 412 543 1088 0.3 82.5 55 67.4 65.7 385 543 1088 0.3 110 55 65.6 64.3 453.8 543 1088 0.3 27.5 68.8 72.1 68.8 426.3 543 1088 0.3 55 68.8 70.1 67.2 398.8 543 1088 0.3 82.5 68.8 65.8 64.3 440 543 1088 0.3 27.5 82.5 65.8 67.1 412.5 543 1088 0.3 55 82.5 63 65.4 © 2019, IRJET | Impact Factor value: 7.211 | ISO 9001:2008 Certified Journal | Page 1387